Quaternary Aluminum Silicides Grown in Al Flux: RE5Mn4Al23-xSix (RE = Ho, Er, Yb) and Er44Mn55(AlSi)237
Nicholas P. Calta; Mercouri G. Kanatzidis; Inorganic Chemistry 52 (2013) 9931–9940; doi:10.1021/ic401659y

data_4335910
_publ_section_title
;
 Quaternary Aluminum Silicides Grown in Al Flux: RE5Mn4Al23-xSix (RE = Ho,
 Er, Yb) and Er44Mn55(AlSi)237
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9931
_journal_page_last               9940
_journal_paper_doi               10.1021/ic401659y
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Al236 Er88 Mn110 Si238'
_chemical_formula_weight         33814.98
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           223
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   21.8208(4)
_cell_length_b                   21.8208(4)
_cell_length_c                   21.8208(4)
_cell_measurement_reflns_used    30886
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.48
_cell_measurement_theta_min      1.86
_cell_volume                     10389.9(3)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'image plate (34 cm diameter)'
_diffrn_detector_area_resol_mean 6.67
_diffrn_detector_type            STOE
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1166
_diffrn_reflns_av_sigmaI/netI    0.0239
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            56227
_diffrn_reflns_theta_full        24.99
_diffrn_reflns_theta_max         24.99
_diffrn_reflns_theta_min         1.87
_exptl_absorpt_coefficient_mu    21.960
_exptl_absorpt_correction_T_max  0.4918
_exptl_absorpt_correction_T_min  0.3082
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details   X-Red32
_exptl_crystal_colour            'metallic silver'
_exptl_crystal_density_diffrn    5.404
_exptl_crystal_description       plate
_exptl_crystal_F_000             15134
_exptl_crystal_size_max          0.061
_exptl_crystal_size_mid          0.045
_exptl_crystal_size_min          0.002
_refine_diff_density_max         1.312
_refine_diff_density_min         -1.712
_refine_diff_density_rms         0.273
_refine_ls_extinction_coef       0.000014(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.445
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     149
_refine_ls_number_reflns         1661
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.445
_refine_ls_R_factor_all          0.0603
_refine_ls_R_factor_gt           0.0502
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0175P)^2^+232.5937P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0712
_refine_ls_wR_factor_ref         0.0730
_reflns_number_gt                1510
_reflns_number_total             1661
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic401659y_si_001_1.cif
_cod_data_source_block           cubic
_cod_database_code               4335910